15 Applications of Thermoplastic Elastomers 15.1 Introduction Since the commercial introduction of thermoplastic elastomers (TPEs) in the late 1960s, about 50 manufacturers of different sizes have entered the field . Thermoplastic polyurethanes (TPUs) were the first TPEs used in the United States and their main applications were automotive exterior parts (bumpers) and shoe soles. Styrenic block copolymers gained rapidly market shares from TPUs in footwear and also established themselves in adhesives and sealants . Olefinics (TPOs) replaced TPUs in automotive sight shields and filler panels and were accepted in wire and cable industry and in hose . By 1983, worldwide TPE demand had reached 421,000 metric tons; its share in the United States was 148,000 tons, 199,800 tons in Western Europe, and 73,900 tons in Japan [3, 4]. During the 1980s there was a rapid growth of use of TPEs in automotive, footwear, wire and cable industries, and adhesives. By the end of 1980s they captured nearly 18% of the U.S. market for medical goods . Total current worldwide annual market demand as pointed out in Section 1.2.6 is about 2,300,000 metric tons and growing at a rate of approximately 6% per year. The TPE market in general, and in the United States in particular, is gradually attaining commodity status, affecting a slew of changes in terms of price and profit margin. Current prices of the base (not compounded) TPEs at moderately large volumes (300,000–500,000 pounds annually) are typically in the $1.50–2.50 per pound range for most grades but may be considerably higher for specialty grades. Given the current raw material situation, the prices will probably grow continuously. Compounded materials are in general less expensive since in most cases the added components used in the compound, such as fillers and/or plasticizers (oils) are less expensive than the base polymer used. Another factor entering the cost picture is the volume cost that frequently favors polymers with low density. In fact, what is very important is the performance/price ratio. This ratio often enters the decision process as to what material to use for a given application. A very simplified chart (Fig. 15.1) attempts to show qualitatively the price and performance ranges for the most widely used TPEs.
Figure 15.1. Approximate ranges of performance vs cost for commercial TPEs (not to scale).
The ability of TPEs to exhibit good flow properties upon heating and then solidifying upon cooling allows the manufacturers to use highly productive thermoplastic processing equipment, such as injection molding, extrusion, and blow molding for the production of elastomeric articles. This eliminates the complicated and costly intensive mixing and vulcanization steps typical for conventional rubber technology. This means reduced labor expenses and increased output. Moreover, the scrap can be reground and reused in virgin materials. Since there are numerous types of TPEs, they cover a wide range of applications, from replacement of conventional vulcanized rubber to special adhesives and sealants. Some of the TPEs in contrast to conventional rubber are very pure and are therefore suitable for medical applications and for articles that come in contact with food. The only case where TPEs have weakness is their service temperature, which depends on their melting point. This can be mitigated by cross-linking, but this reduces the possibility of their recycling. The following sections discuss specific applications of individual types of TPEs.
15.2 Applications for Styrenic TPEs The balance between properties and processability typical for styrenic TPEs leads to focusing on unique applications in addition to the replacement of general-purpose rubber. Styrenic block copolymers are rarely used as neat polymers and can be readily mixed with other polymers, oil, and fillers, which allow versatile tuning of product properties. In most 281
cases the compounded material contains less than 50% of the block copolymer . Formulated styrenic TPEs have several major applications: (1) (2) (3) (4) (5)
Replacement for vulcanized rubber; Adhesives, sealants and coatings; Polymer blends; Bitumen modification; Viscosity index improvers for lubricating oils; (6) Modifiers for thermosets.
Styrene block copolymers can be compounded to produce materials that enhance grip, feel, and appearance in applications such as certain automotive parts (Figs 15.2–15.6), tools (Figs 15.7–15.10), electrical insulation (Fig. 15.11), and molded technical parts, such as plugs (Fig. 15.12), knobs (Fig. 15.13), in personal hygiene (Fig. 15.14), consumer goods (Figs 15.15–15.19), toys, packaging, and others.
The 2002 U.S. styrenic block copolymer demand reported in 2003  was estimated at 647 million pounds, with 30% being in adhesives and sealants, 22% in asphalt modification, 13% in polymer modification, 13% in roofing, 4% in fibers, 3% in consumer products, 3% in footwear, and 12% in other applications. 15.2.1 SBCs as Replacement of Vulcanized Rubber
Styrenic block copolymers used for these applications are mainly styrene-butadiene-styrene block copolymers (S–B–S) and styrene-(ethylenebutylene)-styrene block copolymers (S–EB–S) types compounded to the desired specifications. The compounding ingredients used for that purpose are polystyrene (PS), polypropylene, polyethylene, ethylene-vinyl acetate, oils, and miscellaneous fillers (see Section 5.2.5). Typical applications of compounded styrenic block copolymers are shoe soling, milk tubing, sound deadening materials, grips, wire and cable insulations, flexible automotive parts , automotive parts, sporting goods, parts for construction, as well as molded and extruded industrial goods. Specialized compounds based on S–B–S and S–EB–S are processed into blown or extrusion cast films including heat shrinkable films . Such films are very soft and flexible, exhibit low hysteresis, and low permanent set. Because of their purity they can be used in contact with skin and with certain foods. Solutions of blends of S–EB–S and oils can replace natural rubber latex in the manufacture of dipped articles such as surgeon’s gloves, condoms, etc. . The finished products do not cause allergic reactions as do those made from natural latex and have a much higher resistance to oxygen and ozone due to the saturated center block in the copolymer.
Figure 15.2. Automotive parts (Courtesy PolyOne Corporation).
Figure 15.3. Door handle seal (Courtesy Vi-Chem Corporation).
Figure 15.7. Hand grinder (Courtesy Kraiburg TPE Corporation).
Figure 15.4. Auto floor mat (Courtesy PolyOne Corporation).
Figure 15.8. Rake handle (Courtesy Vi-Chem Corporation).
Figure 15.5. Seals (Courtesy Vi-Chem Corporation).
Figure 15.9. Head lamp (Courtesy Kraiburg TPE Corporation).
15.2.2 SBCs in Adhesives, Sealants, and Coatings
Figure 15.6. Parts interior collage (Courtesy Vi-Chem Corporation).
The use of SBCs in adhesives and sealants is the major segment of their applications (see Section 15.2). A large amount of SBCs is used in hot-melt adhesives, although some adhesives are produced by dissolving them in solvents, taking advantage of their low solution viscosity. The end products
Figure 15.10. Self-inking stamp (Courtesy Kraiburg TPE Corporation).
Figure 15.13. Knobs (Courtesy RTP Company).
Figure 15.11. Power cords (Courtesy Teknor Apex Company).
Figure 15.14. Toothbrush handles (Courtesy PolyOne Corporation).
Figure 15.12. Plugs (Courtesy Vi-Chem Corporation).
are tapes, labels, adhesive fasteners etc. Different types of SBCs are used in different adhesive applications : Styrene-isoprene-styrene block copolymers (S–I–S) and (S–B–S) types having unsaturated elastomeric midblock can be formulated to provide good pressure sensitive adhesives (PSAs). Because
Figure 15.15. Soft shoe inserts (Courtesy Teknor Apex Company).
Figure 15.18. Cooler (Courtesy GLS Corporation).
Figure 15.16. Tongue exerciser (Courtesy Kraiburg TPE Corporation).
Figure 15.19. CD Case (Courtesy GLS Corporation).
Figure 15.17. iPod (Courtesy GLS Corporation).
of the unsaturation, the addition of stabilizers is required. Possible applications are pressure sensitive tapes and labels, contact adhesives, hot-melt adhesive adhesives, construction adhesives and mastics. Styrene-(ethylene-butylene)-styrene (S–EB–S) and styrene-(ethylene-propylene)-styrene block copolymers (S–EP–S) have saturated midblock, exhibit high resistance to degradation by heat, ozone, and ultra violet (UV) light, and have high
tensile strength. These SBC types can be processed at higher temperatures than the others. Possible applications are hot-melt adhesives with long pot life, sealants, and coatings exposed to UV. Styrene-(ethylene-butylene)-styrene copolymers grafted with maleic anhydride have saturated midblocks, good adhesion to polar substrates and can be cross-linked via condensation reactions. These types can act as compatibilizers in multipolymer formulations. Main adhesive application is in structural adhesives, sealants, and PSAs. Polyisoprene-based star block copolymers and S–EB–S block copolymers with high proportion of 1, 2 isomer have been developed. These elastomers can be cross-linked when applied to the tape . This process gives the adhesive improved solvent resistance, which is important for applications in masking tapes . 22.214.171.124 Solution Behavior of SBCs 126.96.36.199.1 Solvents for SBCs The domains and the elastomer blocks can be dissolved in suitable solvents to give solutions of SBCs. The removal of the solvents causes the domains to become hard and glass-like again, and the polymer again acts like a conventional vulcanized rubber. The polymers can be dissolved in many single solvents, such as toluene, and in many solvent blends, such as hexane/methyl ethyl ketone (MEK). In contrast to the usual plastics and rubbers, which have only a single phase, SBCs have two phases. In order to form a true solution, the solvent system must be capable of dissolving both of these phases. Dissolving the PS end-blocks unlocks the network, permitting separation of the solvated rubber blocks. Since SBCs are relatively low in molecular weight, they produce solutions with lower viscosity or with higher solids content relative to solutions of other rubber polymers. Many inexpensive hydrocarbon solvents and some nonhydrocarbon solvents will dissolve both phases. If blends of solvents are used, an even wider variety of solvent systems may be considered. Viscosity, as well as other properties, can be adjusted by the choice of solvent or solvent blend, in accordance with properties desired in the final product. In selecting solvents for SBCs, the solubility parameter () is a useful tool, particularly when working with hydrocarbon solvents. A hydrocarbon polymer will usually dissolve in those hydrocarbon solvents with solubility parameters close to that of the polymer itself. In general, the higher the molecular weight
of the polymer, the closer the solubility parameters must be matched. The relationships involved in the solubility parameter concept are less definite with oxygenated and halogenated compounds, where polar and hydrogen bonding forces become increasingly important. Even in these cases, however, solubility parameters can aid in correlating and predicting solubilities. Viscosity of an S–EB–S grade in various solvent systems is in Table 15.1. Dilute solutions tend to be Newtonian in nature. As concentration increases, solvated domains begin to form in solution just as in the final product. Thus, more viscous solutions become nonNewtonian, particularly when compounded with higher molecular weight polymers . 188.8.131.52.2 Effect of the Addition of Resins and Oils When blended with SBCs, resins improve adhesion, peel strength, shear strength, and reduce solution viscosity. They also help to compatibilize other additives with the block copolymers. High softening point resins which associate with the PS end-blocks increase tensile strength and hardness at a given concentration. An initial yield point in the stress–strain response often results when this type of resin is used. Table 15.1. Viscosity of S–EB–S in Various Solvent Systems (20% Solids) Solvent(s) Heptane Heptane/Acetone Heptane/PCBTF
Solvent Ratio (wt/wt)
Notes: p-chlorobenzotrifluoride. b Tertiary butyl acetate. Source: Kraton® Brochure K0388 bBRa0U, Kraton Polymers LLC, Houston, TX, June 2003. a
Liquid or low softening point resins, which associate with the midblock, can be used to soften the final product, to lower tensile strength, and to increase elongation. Oils have a similar effect. Since four different elastomeric midblocks are typically used in SBCs, the added midblock associating resins and oils must be chosen to be compatible with the particular rubber used in each polymer. Examples of compatibility of a variety of resins and plasticizers with the various midblock elastomers and with the PS end-blocks are shown in Table 15.2. Resins that associate with both phases usually give plasticized products of lower strength, while those that associate with neither phase may result in inhomogeneous and sometimes brittle products. 184.108.40.206 Examples of Applications 220.127.116.11.1 Pressure Sensitive Adhesives Pressure sensitive adhesives are the major end use for SBCs. The adhesive compounds are applied frequently as hot-melts, although solvent application is also used taking advantage of the low viscosity of their solutions (see Section 18.104.22.168). The tack formulations are based on the combination of the polymers with tackifying resins and/or oils (see Section 22.214.171.124). The resins soften the elastomeric phase, which allows the adhesive conform to the substrate in the bonding (slow stage). They also adjust the glass transition temperature of the elastomeric phase, which causes the stiffening of the adhesive layer and resisting the removal of the adhesive Table 15.2. Compatibility of Various Resins and Plasticizers with SBC Segments Additive
Compatible with Segments
Synthetic Polyterpenes (Polymerized C5 Resins)
Hydrogenated Rosin Esters
Saturated Hydrocarbon Resins
Low Molecular Weight Polybutenes Source: Reference .
from the substrate (fast stage). Hot-melt PSAs are mostly based on softer grades of SBCs, such as S–I–S, while solvent based adhesives are frequently prepared from S–B–S and S–EB–S block copolymers using suitable solvents. 126.96.36.199.2 Sealants Sealants are either hot-melts or solvent based and prepared mainly from S–EB–S block copolymers. Diblock polymers are often used in sealants because they reduce the viscosity of the hot-melt product or allow the formulation of a solventbased sealant to be made with higher solids content. Other components of a sealant formulation are resins, oils (plasticizers) and fillers, unless a clear sealant is required. Styrenic block copolymers-based hot-melt sealants are used in many manufacturing processes, sometimes applied by robotics  and can be processed also as foamed products and as formed-in-place gaskets. Solvent-based sealants are mostly used in construction industry . 188.8.131.52.3 Coatings Protective coatings are formulated in a similar manner as adhesives but in many cases they contain large amounts of fillers and UV protective additives (UV stabilizers and titanium dioxide). Such coatings are used on roofs and other outdoor surfaces. Other applications are strippable temporary coatings and in chemical milling of metals . 184.108.40.206.4 Oil Gels Oil gels are primarily blends of oil and gelling agents. The oil comprises the majority of the blend and can be naphthenic or paraffinic processing oil, a mineral oil, a synthetic product such as a polybutene, or a silicone. Gelling agents include waxes, fumed silica, fatty acid soaps, and SBCs. The gelling agent content is usually less than 10%. Products, which range from strong elastomers to weak gels and even greases, can be formulated. Oil gels can be used for sealants, lubricating greases, strippable coatings, corrosion protection, binders, etc. . An example is a blend of S–EB–S (typically 5% by weight), a large amount of mineral oil (90%), and the remainder of wax (5%) are used as cablefilling compounds for “bundled” telephone cables [17, 18]. Their function is to prevent water intrusion and wicking. A potential application of such gels is in toys, hand exercising grips, soft pads, etc. .
220.127.116.11.5 Viscosity Index Improvers Styrene-(ethylene-propylene) (S-EP) diblocks and certain star block copolymers [19, 20] are used in small amounts in motor oils. The typical amount of changing SAE 10 weight oil into multigrade oil (10/30 or 10/40) is 0.7–2.0 wt%. At low temperatures the SBC molecules are compact and cannot crystallize in oil, thus allowing an easy starting of the engine. At high temperatures, the SBC molecules expand in the oil thus maintaining its viscosity and maintaining thick enough lubricating film on bearings and other parts of the engine and reducing wear . 15.2.3 Blends of SBC with Other Polymers
Styrenic block copolymers are compatible with a large number of polymers. Many blends of SBCs with other polymers yield materials with improved properties when compared to the original polymers and this applies to both thermoplastics and thermosets. The improved properties are impact resistance, tear strength, stress crack resistance, low temperature flexibility, and elongation. Some effects are shown in Table 5.2 (Section 5.2.5). Examples of such blends and their properties are discussed below. 18.104.22.168 Blends of SBCs and PS
The most widely used application is improving impact resistance and crack resistance of clear PS for cups, food containers, and films. Others are further increase of impact resistance of impact resistant PS, creating a super-impact PS, and restoring impact resistance of PS after flame retardants were added to it .
Figure 15.20. Films (Courtesy PolyOne Corporation).
polycarbonate  and as impact modifiers in polyamides and polyesters . 22.214.171.124 Blends of SBCs with Thermosets
Special types of PS-elastomer block copolymers were developed for the use in sheet molding compounds (SMCs). Sheet molding compounds are thermosetting compounds that contain unsaturated polyesters, styrene monomer, chopped fiberglass, and fillers and are used for rigid parts in automobile exteriors. The addition of the special type of SBCs is used to control shrinkage during cure. The final products have improved surface appearance and better impact resistance [25, 26].
126.96.36.199 Blends of SBCs and Polyolefins
The addition of SBCs improves low-temperature impact resistance of polypropylene. Blends of SBC and polyethylene are used mainly in blown and cast films (Fig. 15.20). The resulting film has improved tear strength and impact resistance . Blends of SBCs, particularly of S–EB–S and olefins (polypropylene and polyethylene) are used in a variety of applications, including “soft touch” and ultrasoft materials. Examples of applications of blends of SBCs with polyolefins are illustrated by Figs 15.21–15.23. Other useful blends of SBCs are with engineering thermoplastics such as polyphenylene oxide  and
Figure 15.21. Grips on pens (Courtesy Teknor Apex Company).
Styrene block copolymers absorb the “oily components” from the bitumen increasing their volume to as much as 10 times the polymers volume. The network formed by the styrene domains is inflated but can remain intact throughout the binder giving it elastic properties over a much wider temperature range. This reduces the viscous behavior at high temperature and the brittle behavior at low temperature . Modified asphalt is used for road pavements , for chip seals (used to hold the aggregate together when road is resurfaced), slurry seals, and road crack sealants. Other applications are flat rolled roofing, shingles, pressure sensitive modified asphalt membranes, hot mopped asphalt, and other waterproofing applications [29, 30].
Figure 15.22. Super soft clear gel (Courtesy Teknor Apex Company).
15.3 Applications of Thermoplastic Vulcanizates (TPVs) and ETPVs 15.3.1 Introduction
Introduced commercially in 1981, the TPVs had found annual worldwide aggregate applications in excess of 20 million pounds (9,000 metric tons), by the mid-1980s, with more than one thousand different commercial uses . The current estimated consumption (2004) is 162,000 metric tons with projections to 2014 to be 332,000 metric tons . 15.3.2 Comparison of TPVs and Thermoset Rubber Materials
Figure 15.23. Swim fins (Courtesy Teknor Apex Company).
15.2.4 Modified Asphalt
The modification of asphalt is one of the fastest growing applications for PS block copolymers. Styrene block copolymers are added at amounts less than 20% of the total weight and in some cases even as little as 3%.
Direct comparison of performance and costs of main grades of TPVs and thermoset elastomers have properties somewhere in the range of EPDM, CR (polychloroprene), and CSM (chlorosulfonated polyethylene-Hypalon® ) . Another comparison , which charts various thermoset and TPE materials according to their service performance in hot air and the swelling in IRM 903 (ASTM #3 Oil) at this temperature positions the EPDM/EPM-based TPVs between CR, EPDM, and CSM and NBRbased TPVs near nitrile and epichlorohydrin rubber materials. Thus the former is a logical candidate for applications requiring a broad spectrum of properties of special purpose elastomers (CR, EPDM, CSM) and the latter for applications requiring an oil resistance comparable to that of NBR . DuPontÔ ETPV withstands temperatures up to 160˚ C (320˚ F), retains flexibility down to 40˚ C ( 40˚ F) and resists oil, grease and chemicals,
which makes it suitable for a variety of automotive applications. 15.3.3 Commercial Applications of TPVs
Because of the wide spectrum of properties of TPVs, they found applications in many areas such as
Automotive Hose, tube, and sheet Mechanical rubber goods and consumer goods Architectural and construction Electrical and electronic Medical and food contact.
188.8.131.52 Automotive Applications
The automotive industry was the first to utilize the performance/cost advantages of TPVs, since these materials are well suited to the specific needs and trends of that industry. Significantly more than half of the rubber materials used in an automobile is found in non-tire uses . The most important factors determining the automotive applications are:
Figure 15.24. Drive shaft boot (Courtesy Zeon Chemicals LP).
Steadily increasing under-the-hood temperatures Continuing emphasis on safety and reliability Quality and cost of rubber articles Ease of installation of the rubber parts into the vehicle subassembly. The currently used components manufactured by melt-processing techniques, such as injection molding, blow molding, simple and crosshead extrusion are, for example [31, 35]:
Convoluted boots protecting rack and pinion steering gear assemblies Drive shaft boot (Fig. 15.24) Window seals Hose coverings Air inlet duct covers (Fig. 15.25) Vibration dampeners Gaskets and seals (Fig. 15.26) Ignition cable coverings Body plugs Steering column collar (Fig. 15.27).
Figure 15.25. Clean air intake duct (Courtesy Zeon Chemicals LP).
DuPontÔ ETPV has been used in automotive ducts (Fig. 15.28), brake hoses (Fig. 15.29), spark plug boots (Fig. 15.30), seals, body plugs, and others. 184.108.40.206 Hose, Tubing, and Sheet
The main advantage of this group of products is that they can be manufactured by simple meltprocessing methods such as extrusion and calendering and no vulcanization is required after the processing. The widest application of TPV sheeting is a roofing membrane that can be easily seamed on site by heat sealing. Other extruded or calendered sheets are used for die-cut seals and gaskets.
Figure 15.26. Dust seal (Courtesy Zeon Chemicals LP).
Figure 15.29. ETPV automotive brake hose (Courtesy DuPont).
Figure 15.27. Automotive steering column collar (Courtesy Solvay Engineered Polymers Inc.). Figure 15.30. Spark plug and ignition coil boots (Courtesy DuPont).
such as polypropylene, polyethylene. Typical examples are: hydraulic (wire braid) hose, agricultural spray, plant air–water, and mining hose, and industrial tubing . Tubing extruded from stiffer grades can be used as a hose without reinforcement for less demanding applications. 220.127.116.11 Mechanical Rubber Goods and Consumer Goods Figure 15.28. ETPV automotive fuel vent tube (Courtesy DuPont).
Extruded tubing from TPV can be used as innerliner or jacket of hose, or both for hose reinforced by textile or metal mesh. In hose applications the TPEs can be combined with compatible thermoplastics,
This very large group of products comprises the multitude of applications such as parts of industrial equipment, household appliances, recreational and sporting goods, tools, and other; these are manufactured mainly by injection molding, blow molding, and extrusion. Examples are seals, gaskets, valve seats, bushings, grommets, appliance feet, caster wheels injection molded over thermoplastic core,
torque couplings, vibration isolators, suction cups, caps, rollers, extruded profiles, bumpers, housings, convoluted bellows, housings, shields, toys, ski pole grips, and soft-feel tool grips, foamed profiles and sheets. Examples of such applications are in Figs 15.31–15.38. 18.104.22.168 Architectural and Construction
Thermoplastic vulcanizates are widely used in expansion joints, roofing, flooring, weather seals around doors, windows and other exterior openings in large commercial buildings, such as shopping centers, warehouses, office buildings, high-rise apartments, and hotels. Specific examples are soft extruded window glazing material and metalreinforced weather stripping. Applications requiring fire resistance can employ special TPV grades formulated with reliable flame retardants .
Figure 15.32. Sippy Cup (Courtesy GLS Corporation).
22.214.171.124 Electrical and Electronics
Electrical properties of TPVs  indicate that TPVs can be used as primary insulator, jacketing material, or both. Wire and cable insulations are most widely fabricated by crosshead extrusion over a metal conductor or over its dielectric insulation. Electrical connectors, plugs, and insulators for electrical and electronic assemblies are mainly produced by injection molding, often with metal inserts . Other applications are in computer hardware,
Figure 15.33. Hand drill (Courtesy GLS Corporation).
Figure 15.31. Camera (Courtesy GLS Corporation).
Figure 15.34. Bicycle grip (Courtesy Teknor Apex Company).
Figure 15.35. Grip on iron (Courtesy Teknor Apex Company).
Figure 15.37. Grips on screwdrivers (Courtesy Teknor Apex Company).
Figure 15.36. Syringe seal (Courtesy Teknor Apex Company).
telephones, electronic appliances, and office equipment. An example of electrical application is a conductive cap (Fig. 15.39). 126.96.36.199 Medical and Food Contact
Thermoplastic vulcanizates based on EPDM are suitable for use in direct contact with foods, beverages, pharmaceuticals, and living tissues. These applications employ grades approved by U.S. Food and Drug Administration. Medical
Figure 15.38. Soft touch applications (Courtesy Teknor Apex Company).
applications include drug vial stoppers, syringe plunger tips, aerosol valve seals, medical tubing, liquid dispenser pump diaphragms, and nursing bed sheets.
Figure 15.39. Conductive TPE cap (Courtesy RTP Company).
15.4 Applications of Thermoplastic Polyolefin Elastomers (TPOs) Polyethylene-poly(a-olefin) block copolymers have rather complex morphology; the distribution, size, and shape of both soft and hard phases determine the properties of the copolymer. The polypropylene phase is almost always continuous and the rubber phase may be either continuous or discrete, depending on the amount of rubber in the compound relative to polypropylene . The copolymers are very flexible at low temperatures; however their upper service temperature is rather low, suggesting that the polyethylene segments are rather short. The lower service temperature can be near 80˚ C ( 112˚ F) the upper service temperature up to 140˚ C (284˚ F) for short-term exposure, and 105˚ C (221˚ F) for long-term exposure. They have some resistance to oils and solvents . Commercial TPO materials are available in the hardness ranging from 65 Shore A to 70 Shore D. Thermoplastic polyolefinics are supplied as pelletized compounds developed for specific applications and processing methods. They are processed mainly by injection molding, extrusion, injection blow molding, and vacuum forming, and as blown film . Thermoplastic polyolefinics products are used in a variety of applications with major market areas being
Automotive applications are their largest market. Thermoplastic polyolefinics are used in many soft, durable exterior parts to replace sheet metal, giving parts that are not easily damaged by minor collisions, including bumper covers, bumper end caps, body side cladding, body side molding, air dams, fairing pieces, fender liners, rocker panel covers, rub strips, scuff plates, sight shields, stone deflectors, wheel well moldings, grills, and valance panels. Parts in the engine compartment include heating air ducts, conduits, grommets, hood seals, and firewall pads. In the interior, the applications include air bag covers, instrument panels, knee bolsters, glove box doors, door panels, door inserts, and soft skins laminated to polyolefin foam for interior trim. Examples of automotive applications are in Figs 15.40–15.44. 15.4.2 Wire and Cable
Wire and cable applications include flexible cords, battery booster cables, appliance wires, low voltage wire, control cables, hook-up wire, submersible pump cable, and cable jackets. Excellent electrical properties, ozone resistance, and water resistance are the main attributes in these applications . Wire and cable products include both standard and flame retardant grades. 15.4.3 Mechanical Goods
The mechanical goods market is very diverse and many applications include small molded parts where TPO compounds replace vulcanized rubber. For example, they replace butyl rubber in molded parts for electrical applications, CR in bumpers, seals, and electrical plugs. Other parts include gaskets, pump impellers, molded feet, and wheels. The
Automotive Wire and cable Mechanical goods.
Figure 15.40. Automotive bumper fascia and grille surround (Courtesy Solvay Engineered Polymers Inc.).
Figure 15.41. Mold-in-color metallic exterior wheel opening trim (Courtesy Solvay Engineered Polymers Inc.).
Figure 15.44. Thermoformed all terrain vehicle deck (Courtesy Solvay Engineered Polymers Inc.).
Figure 15.42. Automotive instrument panel-upper (Courtesy Solvay Engineered Polymers Inc.).
Figure 15.45. Clean room scanner (Courtesy RTP Company).
Figure 15.43. Automotive interior, roof pillar cover (Courtesy Solvay Engineered Polymers Inc.).
advantages of TPO in all these applications is that production and postconsumer scrap can be recycled and that production cycles for TPO parts are much shorter. Examples are in Figs 15.45 and 15.46. Extruded products in the mechanical goods field, where TPO is used are sheets, films (extruded and blown), weather strips, profiles, tubing, hose, etc.
Figure 15.46. Electric probes (Courtesy RTP Company).
15.4.4 Other Applications
Other applications include transmission belts, specialty conveyor belts, housewares, toys, recreational and sporting goods, luggage handles, shoe
Figure 15.48. Cutting board (Courtesy Vi-Chem Corporation). Figure 15.47. Bicycle hub (Courtesy RTP Company).
soles, drum covers, garden hose, spatulas, sealants, tapes, and hot-melt adhesives. Examples are in Figs 15.47 and 15.48.
15.5 Applications of Melt-Processible Rubber (MPR) Single-phase MPR introduced in 1985  produces parts that have the appearance and feel and perform like those made from vulcanized rubber. At the same time, it offers an unusual combination of resistance to heat, oil and chemicals, and weathering. Depending on grade, the brittleness temperatures range typically from 87˚ C ( 124˚ F) and the upper continuous service temperature is typically 120˚ C (248˚ F) . Another valuable attribute of MPR is a high coefficient of friction; well over 1.0, which is almost double of that of other TPEs such as styrenics and TPVs of similar hardness . Since most commercial MPR grades contain from 9% to 20% of chlorine, they are flameresistant enough to pass UL-94 HB (horizontal burning) rating as sold and with the addition of a suitable flame retardant they can attain the UL-94 V-0 (vertical burning) rating . As supplied, MPR grades are static-charge dissipative and can be made semi-conductive by
compounding them with conductive fillers. These properties made them suitable for applications where static discharge could lead to explosions of dust or solvent vapors (conveyor belts or conveyor hose) or to damage of electronic components. Melt-processible rubber can be processed in plastic and certain modified rubber processing equipment and has been used in a variety of applications, including flexible tubing, molded parts, seals, gaskets, weatherstripping, reinforced hose, wire and cable jacketing, and coated fabrics. Principal market segments for MPR are extruded and molded goods, and sheeting. The most widely used processes are extrusion, injection molding, blow molding, and compression molding [41, 42]. 15.5.1 Industrial Hose
Melt-processible rubber is suitable for the use in tube and cover for general purpose, weather resistant, oil resistant, chemically resistant hose, and hose with static dissipative or semi-conductive properties (see above). 15.5.2 Automotive
The outstanding weathering resistance of these materials, coupled with durable outstanding elastic properties makes them the primary choice for automotive glass seals. Other automotive components made from MPRs are fuse holders, interior trim, knobs, grips, steering wheels, outer belt strip
moldings , fuel lines, boots, bellows, dust covers, etc. Examples of automotive applications are in Figs 15.49 and 15.50. 15.5.3 Wire and Cable
In general, MPR is used mostly for some lowvoltage (£600 V) applications, where toughness, environmental endurance, and rubbery quality are required. Typical applications are flexible cord applications, welding cable with excellent spark burn-through resistance and as jacketing in highervoltage construction to provide durable protection to primary insulation. 15.5.4 Elastomeric Sheeting
Sheeting from MPR can be fabricated either by sheet extrusion or by calendering. Calendered sheets, unsupported or fabric reinforced can be easily produced in a single pass without blisters or defects. If desired, the sheets can be embossed by embossing rolls while the stock is still warm . Typical application of sheeting is as roofing membranes, pit and pond liners.
Figure 15.50. Hummer latch (Courtesy Advanced Polymer Alloys).
15.5.5 Molded Goods
In this market, MPR is being used for molded parts in industrial, automotive original equipment manufacturer (OEM) equipment, automotive aftermarket, appliances, and oil field outlets. The parts are predominantly produced by injection molding and blow molding and may include articles with metal inserts or parts prepared by bonding rubber to metal by specialized adhesives. Of particular importance are “soft touch” molded articles, used
as grips of tools, grips, push buttons, and parts of instruments and hand-held devices as well as handles and other flexible parts of household appliances. Many of these are made by overmolding of rigid components by a soft-touch MPR materials. In some cases an entire device is encased in MPR protective layer for comfortable use and protection from workplace hazards such as drops and fluid spills . Examples are in Figs 15.51–15.53. 15.5.6 Fabric Coating
Figure 15.49. Wind lace (Courtesy Advanced Polymer Alloys).
In fabric coating, MPR has replaced vulcanized rubber in some applications, where the unusual hand and drape of MPR-coated fabric are of interest. An example of this application is as inner and outer coating on fabric used to make huge inflatable pillow-tanks for environmental protection. Such tanks are stored on the decks of oil tankers and can be deployed in case of emergency to transfer the oil from the tanker and be launched into the sea. The capacity of such pillow tank can be as much as 20,000 cubic meters (706,300 cf) . Other application in this area is to modify PVC compounds to reduce sheen and add to drape and hand .
Figure 15.53. Stream light (Courtesy Advanced Polymer Alloys). Figure 15.51. Buck knife handle (Courtesy Advanced Polymer Alloys).
light in color, they can be easily colored by the addition of a variety of inorganic and organic pigments and color concentrates and it is possible to obtain bright colors as well as variety of special effects, such as metallic, pearlescent, thermochromic, etc. Other applications are architectural window and door seals, home and commercial irrigation systems, agricultural equipment, variety of seals, telephone and calculator keypads, grips on cameras and more. Architectural applications of MPR are in Figs 15.54 and 15.55.
15.6 Applications of PVC Blends 15.6.1 PVC–Nitrile Rubber (NBR) Blends
Figure 15.52. Drill handle (Courtesy Advanced Polymer Alloys).
15.5.7 Other Applications
Many articles from MPR find applications in the consumer market, including toys. Since the commercial grades are clear or translucent and
Poly(vinyl chloride) and NBR have been blended in different ratios for many years. In blends, where the predominant component is PVC, NBR acts as a true plasticizer and the resulting blends are more rubbery than PVC plasticized with liquid plasticizers (e.g., dioctyl phthalate) but not very elastomeric. In general, NBR with the acrylonitrile contents of 40% is needed to obtain a single phase blend . The NBR can be noncross-linked or pre-cross-linked to different degree. The former yields blends with lower viscosity suitable mainly for injection molding. Pre-cross-linked NBR provides a material with a resistance to compression set and other elastomeric characteristics to be considered a true TPE. It also increases melt viscosity of the blend so that it is more suitable for extrusion and calendering.
When properly formulated, PVC–NBR blends exhibit an excellent resistance to chemicals and to swelling in oils, and a very good abrasion resistance. They can be welded by heat, radio frequency, or ultrasonic methods or bonded by adhesives. Depending on the melt viscosity (see above), they can be processed by injection molding, extrusion, calendering, or extrusion blow molding. Typical articles made from these blends are seals and gaskets, hose tubing and cover, cable jackets, boots and soling, grommets and plugs, and bellows and sleeves.
15.6.2 PVC–Copolyester Elastomer (COPE) Blends
Figure 15.54. Building with MPR curtain wall seals (Courtesy Advanced Polymer Alloys).
Although plasticized (flexible) PVC (FPVC) and COPEs are compatible in wide range of ratios, only such blends where FPVC is used to increase flexibility of COPE are practical, the reason being the high cost of COPE in comparison to FPVC. For the reason of preventing decomposition of PVC during processing only low melting COPEs with about 33% 4GT and melting temperature below 180˚ C (356˚ F) are being used. Typical applications of PVC–COPE blends are as a lower cost alternative to TPUs in hose tubing and cover. Other uses are automotive primary wiring that is more heat resistant than PVC wiring, protective jackets for retractile cords for telephones and domestic electrical appliances that have better memory characteristics than FPVC. Another lower cost alternative to TPU is in sport shoe soling.
15.6.3 PVC–TPU Blends
Figure 15.55. Architectural extrusions (Courtesy Advanced Polymer Alloys).
Most of the TPUs are very compatible with PVC and such blends exhibit only one major glass transition, whose position on the temperature scale is raised with increasing levels of PVC . As it is the case with PVC–COPE blends, most widely used blends are those where PVC is added to TPU to maintain desirable properties of TPU while reducing cost . The main applications of blends of PVC–TPU are in shoe soles and heels. Their main attributes are good wear resistance, good flexibility, good compression set, oil resistance, and reasonable cost. Essentially the materials have better performance than pure PVC but lower cost than pure TPU.
15.7 Application of TPUs 15.7.1 Introduction
Thermoplastic polyurethane elastomers are multiblock copolymers with alternating hard and soft segments. The hard segments (predominantly crystalline) are polyurethanes or polyureas. The soft, elastomeric segments are amorphous and are based on polyesters or polyethers. Each of these types of TPUs has specific attributes (see Section 9.5) that make them useful in a great variety of applications. The ester-based TPUs have excellent tensile strength, load-bearing capacity, and resistance to abrasion, ozone, oxygen, fuel, oils, and solvents. The ether-based TPUs provide excellent low temperature properties and resistance to hydrolysis, and to microbial attack. Thermoplastic polyurathanes with special properties can be obtained by reinforcement or polymer blending. Depending on the structure and additives used in specific compounds, TPUs have the following distinctive properties:
Abrasion resistance Clarity Cut resistance Flexibility Heat sealability Load bearing capacity Low-temperature flexibility Non-marking Oil resistance Toughness Vibration damping.
parts, fuel line hose, timing belts, shock absorbers (Fig. 15.56), bumpers, fender extensions, membranes of hydro-pneumatic suspension system, hatchback strap, side shields, filler panel, fender and quarter panel extension, windshield and closeout lace, valance panel, instrument panel, interior trim, skins of instrument panels (Fig. 15.57), automotive center consoles (Figs 15.58 and 15.59), gear knobs (Fig. 15.60), car keys (Fig. 15.61) gears and assembly line equipment. 188.8.131.52 Hose and Tubing
Examples of the TPU hose and tubing are irrigation hose, garden hose, fire hose, hydraulic hose, sewer hose, fuel line hose for snowmobiles and small gasoline engines, pneumatic tubing for robotics, surfboard lashes and cords, medical tubing. 184.108.40.206 Wire and Cable
Wire and cable applications include seismographic cable, audio wire, camera cable, computer cable, head-set cable, marine cable, welder cable, air gun control cable, communication wire, towing leader, abrasion resistant cable jacketing, plugs (Fig. 15.62), etc.
15.7.2 Commercial Applications
In some applications TPUs are replacing vulcanized rubber , although in majority of cases they are used because of their unique combination of properties. The specific areas, where TPUs are widely used include automotive, hose and tubing, wire and cable, wheels and casters, film and sheet, adhesives, sealants and coatings, and general purpose articles. 220.127.116.11 Automotive
Typical TPU articles in automotive applications are: gaskets, seals, bushings, bellows, steering gear
Figure 15.56. Elastic element for shock absorber (Courtesy Bayer MaterialScience LLC).
Figure 15.59. Gear shifting handle (Courtesy RTP Company).
Figure 15.57. Skins of instrument panels (Courtesy Martin Thomas International).
Figure 15.60. Gear shift knobs (Courtesy Bayer MaterialScience LLC).
Figure 15.58. Auto tamber door (Courtesy Bayer MaterialScience LLC).
18.104.22.168 Wheels and Casters
Examples for these applications are wheels and casters for shopping carts, food service carts, and hospital carts, wheels for inline skates and skateboards, and others.
Figure 15.61. Car key (Courtesy Bayer MaterialScience LLC).
Figure 15.62. Electrical plugs (Courtesy Bayer MaterialScience LLC).
22.214.171.124 Film and Sheet
Thermoplastic polyurethane films and sheets are produced by flat film extrusion, blown film extrusion, or calendering in gauges from approximately 20 mm up to several mm typically using materials with hardness between 60 and 95 Shore A. The films can be laminated to PU foams and textiles and show high puncture resistance . Special grades based on poly(ethylene glycol) soft segments with high water vapor transmission are used for breathable films in the textile industry .
Figure 15.63. Inflatable raft from TPU-coated fabric (Courtesy Merquinsa).
products . An example of an application of clear TPU protective coating on fabric is in Fig. 15.64. 126.96.36.199 Mechanical Goods, Consumer, and Sporting Goods
Thermoplastic polyurethanes are used in drive belts, gaskets and seals (Fig. 15.65), industrial hose and tubing, tire chains, shoe soles and heels, grommets and spring sleeves, bushings and dust caps for supporting joints, wire and cable jackets, overmolded parts with a soft grip, such as handles
188.8.131.52 Adhesives, Sealants, and Coatings
The number of applications of TPUs in adhesives, sealants, and coatings is smaller than rubber replacement and other uses. In adhesive technology, they are applied mostly as hot-melts , although some grades can be applied from solutions in polar solvents, such as MEK of dimethyl formamide. The hot-melts are useful in footwear for attaching soles to the uppers, and in coextrusions, where they are used as tie layers between dissimilar polymers . Thermoplastic polyurethane-based coatings are used mainly for coating fabrics used for inflatable boats (Fig. 15.63), collapsible canoes, life rafts, life jackets, and oil barriers . Coating of individual yarns increases greatly the tenacity of the yarn and protects it again soiling. Special yarns coated with transparent TPU are woven into decorative textiles used in car seats, armchairs, and office chairs . Other applications are shoe lacquers, inks, magnetic tape binders, luggage, gel seats, and artificial chamois
Figure 15.64. Automotive seat from fabric treated with clear TPU coating (Courtesy Bayer MaterialScience).
Figure 15.65. TPU seals (Courtesy Bayer MaterialScience LLC).
of machines, tools, appliances and furniture , sporting goods (frames of ski goggles, ropes for surfboards, parts of ski bindings, studs for sport shoes, and shells of inline skates, golf ball covers), soccer ball covers (Fig. 15.66), tennis racquet components (Fig. 15.67). Grades with hardness greater than 55 Shore D are used in shells for ski boots, utilizing their exceptional scratch resistance, low temperature impact resistance, and low relative sensitivity of stiffness to temperature. Animal identification tags (short-term and long-term tags)
Figure 15.67. Tennis racquet components (Courtesy RTP Company).
are rather unique application for TPU, using grades with 90–95 Shore A hardness based on polyether or polycarbonate soft segments  (Fig. 15.68). An example of a TPU lap station is in Fig. 15.69. 184.108.40.206 Medical Applications
Thermoplastic polyurethanes are compatible with human blood and tissue and therefore can be used in medical devices, such as catheters and tubing [53, 55]. Materials based on methylene diphenyl diisocyanate (MDI) cannot be in contact
Figure 15.66. TPU soccer ball (Courtesy Bayer MaterialScience LLC).
Figure 15.68. Animal tags (Courtesy Merquinsa).
them competitive with chemical resistant and specialty elastomeric materials based on NBR, epichlorohydrin, and polyacrylate. Commercial grades are available in the range of Shore D hardness values from 30D to 82D. Special grades contain UV stabilizers, heat stabilizers, flame retardants, or hydrolysis resistant additives. They can be processed easily by conventional thermoplastic processes like injection molding, blow molding, calendering, rotational molding, extrusion, and meltcasting. 15.8.2 Commercial Applications
Figure 15.69. Lapstation (Courtesy GLS Corporation).
with human tissue for more than 28 days, however TPUs based on aliphatic diisocyanates can be used for longer exposures, even as body implants . 220.127.116.11 Blends with Other Polymers
Blends of TPU with many thermoplastic and elastomers are relatively easy to prepare. The only polymers that show little or no compatibility are non-polar polymers, such as polyolefins . The most widely used blends of TPUs are those with plasticized PVC (see Section 15.6.3) that have good flex life, oil resistance, abrasion resistance, and low-temperature flexibility and are being used in special footwear .
15.8 Application of Thermoplastic Polyether Ester Elastomers 15.8.1 General Properties and Processing
Thermoplastic polyether ester elastomers comprise of alternating hard and soft segments, where the hard segments are crystalline polyester, poly(butylene terephtalate) and the soft (elastomeric) segments are almost always copolymers of terephtalic acid with poly(oxytetramethylene glycol). They are tough materials exhibiting high tear strength, high flex-cut resistance, abrasion resistance, creep resistance, high oil and solvent resistance, and low compression set. At low strains they have a low hysteresis, behaving almost like a perfect spring . Thermoplastic polyether ester elastomers are resistant to hot oils, and this makes
In commercial applications, COPEs can replace a variety of conventional materials, such as metal, cast polyurethanes, leather, and rubber. Within their elastic design range, COPEs offer 2–15 times the strength of vulcanized rubber. Because of that, it is common to redesign rubber parts for one-half to one-sixth the original part thickness and weight. Non-reinforced COPEs also can replace composites of rubber with metal, fibers, and fabric. 18.104.22.168 Automotive Applications
Automotive applications include constant velocity drive joint (CVJ) boots (Fig. 15.70), spoilers, air dams, side moldings, fascia, grills, hinges and locks [59, 60], protective boots in suspension joints, primary pump for automotive fuel lines . In these applications, if needed, the parts are easily painted or sputter chrome coated because of their excellent molded surface and heat resistance. 22.214.171.124 Electrical/Electronic Applications
Electrical/electronic applications include thin wire insulations, retractable coiled cables (Fig. 15.71),
Figure 15.70. CVJ Boot (Courtesy DuPont).
couplings, backup rings for hydraulic piston devices, gears power drive belts, toothed belts for office equipment, pipe clamps, tracks for recreational, farm and military vehicles, railroad draft gear, liner of butterfly valves, power tool handles, heel cushioning system of running shoes, wrist protector for snowboard riders , and many molded articles with high wear resistance, very good flexibility and impact resistance [62, 63]. Examples of such applications are in Figs 15.73–15.76.
126.96.36.199 Other Applications Figure 15.71. Retractable coiled electric cable (Courtesy DuPont).
hermetically sealed units, switches and connectors, panel insulator covers [59, 60, 62]. In fiber optics technology, COPEs are used as the primary coating, secondary coating, buffer tube, and jacket taking advantage of their combination of their mechanical strength and environmental resistance [62, 63]. 188.8.131.52 Extruded and Molded Mechanical Goods
Typical applications for COPEs in this field are specialty hose tube (Fig. 15.72), hydraulic hose and cover with service temperatures 65˚ F to +250˚ F ( 54˚ C to +121˚ C) and 275˚ F (135˚ C) for intermittent use , pneumatic tires (without reinforcement) with a high load-bearing capacity (made by rotational casting). Other products are flexible
Figure 15.72. PVC tubing with COPE lining (Courtesy New Age® Industries Inc.).
An important application of COPEs is in medical devices, where compatibility of the resins with human blood and tissue, their chemical purity and inherent resistance to radiation used for sterilization are key advantages [64–66]. An example for a medical application is an IV bag shown in Fig. 15.77. Higher hardness polyethylene oxide (PEO)based polyether esters exhibit a high water vapor transmission rate and are for that reason used in waterproof, breathable films that are laminated with fabrics and used in the manufacture of outer garments, such as jackets, pants , gloves, tents, footwear  and single-use surgical gowns . Another application of breathable COPE films is in carpet underlay. The film is laminated to the surface of the carpet foam cushion. Such laminate allows easy cleanup of spills by blocking the penetration of the spilled liquids and minimizes the undercarpet moisture buildup by allowing its escape through the film .
Figure 15.73. Spring bed slats (Courtesy DuPont).
Figure 15.74. Power tool handle (Courtesy DuPont). Figure 15.76. Auxiliary spring (Courtesy DuPont).
Figure 15.75. Telescoping trekking pole (Courtesy DuPont).
15.9 Applications of Polyamide TPEs 15.9.1 Introduction
Polyamide TPEs consist of alternating hard and soft segments joined by amide linkages. The hard, crystalline segments are polyamides and the soft, elastomeric segments are polyethers or polyesters. Depending on the type of building blocks used, the products have different properties. They may
Figure 15.77. I.V. bag (Courtesy Eastman Chemical Company).
be as soft as 65 Shore A and as hard as 70 Shore D. The upper service temperature depends on the choice of polyamide segment and can be as high as 200˚ C (392˚ F). Resistance to oils and solvents of these materials is good. These TPEs can be compounded with various resins or additives to alter or enhance their basic properties. Compounding can be used to adjust cost, toughness, flexibility, tack, and resistance to
oxidation and effects of ozone, flame resistance, and other properties. They also can be blended with other polymers in the melt stage to form alloys of unique properties. Resins that are compatible with the polyamide block tend to produce hard materials with no tack, while the addition of resins compatible with the soft ether or ester segments will produce soft, flexible tacky compounds. Polyamide elastomers can be processed by usual melt-processing techniques, such as injection molding, extrusion, blow molding, rotational molding, and thermoforming. To obtain optimal properties the resins have to be dried to have moisture content less than 0.02% before processing and it is recommended that the feed hopper be purged with dry nitrogen to maintain the low moisture level .
Figure 15.78. Air duct (Courtesy Kraiburg TPE Corporation).
15.9.2 Commercial Applications
Because of their high service temperatures, good thermal aging, and chemical resistance, polyamide elastomers can fill the gap between TPUs and silicone-based polymers. This definitely makes them primary candidates for automotive underthe-hood applications and for high-temperature insulations of wires and cables . Their high impact strength, tear resistance, abrasion resistance, low temperature resistance, and resistance to flex fatigue open a great variety of applications in hose and tubing, seals and gaskets, bellows and other molded technical goods, for sporting goods and others.
Figure 15.79. Automotive timing belt (Courtesy Arkema Inc.).
shells of ski boots (Figs 15.80 and 15.81), soles of athletic shoes (Fig. 15.82), soles with studs (Fig. 15.83), protective and decorative layers of skis  and snowboards (Figs 15.84 and 15.85), decorative films for tennis racquets (Fig. 15.86), ski goggles (Fig. 15.87), swimming goggles (Fig. 15.88) footballs, and basketballs .
Typical uses of polyamide TPEs in automobiles are under-the-hood parts, such as fuel systems, hydraulic and pneumatic systems, various functional parts, seals, gaskets, bellows and protective boots (Fig. 15.78), windshield washer tubings, airbag doors, and shock-absorber parts , timing belts (Fig. 15.79), automobile exterior and interior parts . 184.108.40.206 Sporting Goods
The attributes of polyamide elastomers useful for this market are low weight, excellent mechanical properties, particularly resistance to flexural fatigue, flexibility over a wide range of temperatures, very good UV stability, ozone resistance, easy coloring, and good processing. Products in this category are
Figure 15.80. Shell of alpine boots (Courtesy Degussa AG).
Figure 15.81. Shell of telemark ski boot (Source: DPA).
Figure 15.83. Sole of soccer shoes (Courtesy Degussa AG).
Figure 15.84. Protective and decorative layers for snowboards (Courtesy Degussa AG).
Figure 15.82. Sole of athletic shoes (Courtesy Arkema Inc.).
220.127.116.11 Wire and Cable
Polyamide elastomers are used in wire and cable industry, particularly for high-temperature insulations, abrasion resistant cable jackets, and for nonkinking wires. 18.104.22.168 Technical Goods
Hose and tubing (Fig. 15.89), seals and gaskets, conveyor belts, rollers, silent gears (Fig. 15.90),
Figure 15.85. Molding of a snowboard (Courtesy Degussa AG).
Figure 15.89. Paint spray hose (Courtesy Degussa AG). Figure 15.86. Decorative films for tennis racquets (Courtesy Degussa AG).
Figure 15.90. Silent gears (Courtesy Arkema Inc.). Figure 15.87. Ski goggles (Courtesy Arkema Inc.).
applications for electromagnetic interference/radio frequency (EMI/RF) shielding  are typical applications in this category. 22.214.171.124 Medical Applications
Medical applications include catheters, tubing (Fig. 15.91) and breathable membranes, surgical garments, surgical sheeting, baby diapers, adult incontinence articles , and dental floss (Fig. 15.92).
Figure 15.88. Swimming goggles (Courtesy Arkema Inc.).
powder coated parts, waterproof membranes , bellows and boots for different types of equipment [72, 73], flexible couplings, tire chains, wheels, and semi-conductive films used in packaging
126.96.36.199 Other Applications
Specialty grades of polyamide TPEs are used in decorative and protective films for consumer goods , protective gloves (Fig. 15.93), keyboard covers (Fig. 15.94), food packaging (Fig. 15.95), and processing aid for extrusion of TPUs .
Figure 15.93. Protective gloves (Courtesy Arkema Inc.).
Figure 15.91. Oxygen mask and tubing (Courtesy Nycoa).
Figure 15.92. Dental floss (Courtesy Arkema Inc.).
Figure 15.94. Keyboard cover (Courtesy Arkema Inc.).
15.10 Applications of Ionomeric TPEs
physical, mechanical, and rheological properties of the polymers. General characteristics, of ionomerbased systems are enhanced green strength, and high melt viscosity. The high melt viscosity is useful for heat sealing and in extrusion; however, it may be a limitation in injection molding. Other desirable properties are toughness, outstanding abrasion resistance, and oil resistance. The TPEs in this category are based on carboxylated and sulfonated polymers.
Ionomeric elastomers have been developed in late 1950s and introduced in the early 1960s , but their full potential has not been yet realized . The ionomeric aggregation or formation of clusters (large ionic aggregates), or the interaction of the polar groups have major effects on the
tackifiers (aliphatic petroleum resins) to facilitate bond formation on contact . 188.8.131.52 Other Applications
Figure 15.95. Film pouch for cooking noodles (Courtesy Arkema Inc.).
For practical applications, the base polymers are compounded with mineral fillers, plasticizers (mostly process oils), antioxidants, and polyolefins (polyethylene or polypropylene) using conventional rubber mixing equipment. The finished compositions range typically from relatively soft (hardness 70 Shore A) to very hard, semi-plastic materials (hardness greater than 50 Shore D) [74, 75]. The processing conditions for this class of TPEs are similar to those used for flexible PVC . Blends of ionomeric TPEs with other polymers, such as sulfonated EPDM with polypropylene, sulfonated butyl rubber with polypropylene, high-density polypropylene, and SBC, maleated high-density polyethylene with maleated EPDM, and other similar blends usually exhibit synergistic effects on mechanical properties. These are attributed to the formation of interpenetrating networks and/or ionic interaction between the components . 15.10.2 Commercial Applications 184.108.40.206 Adhesives
One of the fast growing applications of ionomeric TPEs is adhesive technology. Ionic ethylene vinylacetate copolymers are used in various hotmelt and solvent adhesive systems . Carboxyl and sulfonate-containing polymers are used for water-based PSAs often combined with emulsified
Sulfonated EPDM is used in shoe soles, garden hose, and calendered sheets, heat-sealable sheeting (e.g., roofing membrane) . Other applications of ionomeric TPEs include packaging films for processed meats and medical packaging, skin packaging for electronic and hardware items, foil and paper coatings of multiwall bags, golf ball covers, roller skate wheels, bowling-pin coating, etc. , coatings to encapsulate diverse materials (e.g., fertilizers or oxidizing chemicals to assure controlled release . Elastomeric ionomers when added at 5–10% level to asphalt greatly improves the performance of asphalt in roofing applications. Relatively low levels of sulfonated EPDM to various thermoplastics, such as polyamide or polypropylene oxide improve their impact resistance . Recently developed products [74, 78, 79] are suitable for kitchenware, trim for small appliances and office furniture as well for automotive interiors (e.g., shifter knobs) and automotive bumpers and fascias . Potential future applications include foams, elastic fibers with high strength, polymer modifiers, coatings, and more .
15.11 Applications of Other TPEs 15.11.1 Applications of Star Block Copolymers
Star block copolymers prepared by anionic methods have been shown to exhibit superior mechanical properties and lower melt viscosities than linear triblock copolymers with the same molecular weight. The star copolymers with low molecular weight arms exhibited low viscosities and were easily processed (see Section 13.1.2). Because of their unique properties, star block copolymers are widely used in specialty applications. Due to their unusual viscosity behavior, they find use as viscosity modifiers, viscosity index improvers, dispersants, and pour point depressants [80–85] and in adhesives and sealants [86–88]. Star polymers with functional terminal groups are efficient cross-linking agents. For example, star polymethacrylates are reported as reinforcing agents for polyurethanes [89–91]. Since polyisobutylene (PIB) star block copolymers exhibit a superior strength  and improved processing
properties compared to their linear counterparts, it is quite possible that they might in the future replace some linear triblock TPEs in certain applications. 15.11.2 Applications of Thermoplastic Interpenetration Networks
Thermoplastic interpenetrating networks (IPNs) are mostly leathery at the temperatures at which they are used. They exhibit a high flexibility, but are not soft and rubbery as many TPEs discussed in other chapters. The value of certain IPNs exhibit nearly constant modulus in the leathery range from Tg of the center block, –60˚ C up to the melt of the semi-crystalline component (typically 200˚ C or slightly higher ). They are suitable materials
Figure 15.98. Mouth guard (Courtesy RTP Company).
Figure 15.96. Overmolded grips (Courtesy Teknor Apex Company).
Figure 15.97. Grip on electrical carving knife (Courtesy Teknor Apex Company).
Figure 15.99. Intermec Handheld (Courtesy RTP Company).
for automobile bumpers, under-the-hood wiring in automobiles, etc. . 14. 15.11.3 Applications of Special Blends and Proprietary Compounds
Some companies develop specialized compounds based on standard TPEs, their blends or blends with other polymers or use proprietary processes for their preparation. Such materials have often unique properties, such as exceptional softness, unique feel, high resistance to wear, resistance to high temperatures, clarity etc. Examples of such applications are in Figs 15.96–15.99.
References 18. 1. Holden, G., Understanding Thermoplastic Elastomers, Hanser Publishers, Munich, 2000, p. 75. 2. School, R., in Handbook of Thermoplastic Elastomers, 2nd edition, chapter 9 (Walker, B. M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York, 1988, p. 287. 3. School, R., in Handbook of Thermoplastic Elastomers, 2nd edition, chapter 9 (Walker, B. M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York, 1988, p. 290. 4. Chem Systems Inc., Data from Process Evaluation/Research Planning Study, 1985. 5. Carew, R., Paper Presented at Business Opportunities in Biomaterials and Implants, Minneapolis, MN, May 28, 1986. 6. Holden, G., and Hansen, D.R., in Thermoplastic Elastomers, 3rd edition, chapter 19 (Holden, G., Kricheldorf, H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 499. 7. Plastics News, January 27, 2003. 8. Holden, G., and Speer, V.H., Automobile Poly. Design 8(3), p. 15 (1988). 9. Technical Bulletin SC:1105-90, Shell Chemical Company, Houston, TX, 1990. 10. Buddenhagen, D.A., Legge, N.R., and Zschenschler, G., U.S. Patent 5,112,900 (March 12, 1992, to Tactyl Technologies). 11. Publication K0378 VPR, Kraton Polymers, May 2003. 12. Ericson, J.R., Adhesive Age 29(4), p. 22, (1986). 13. Holden, G., and Hansen, D.R., in Thermoplastic Elastomers, 3rd edition, chapter 19 (Holden, G., Kricheldorf, H.R., and Quirk,
26. 27. 28. 29.
R.P., Eds.), Hanser Publishers, Munich, 2004, p. 506. Solution Behavior of Kraton® Polymers, Fact Sheet K0276, Kraton Polymers Houston, TX, June 2002. Holden, G., and Hansen, D.R., in Thermoplastic Elastomers, 3rd edition, chapter 19 (Holden, G., Kricheldorf, H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 507. Oil Gels, Kraton® Styrenic Block Copolymers in Oil Gels, Fact Sheet K0026 Global, Kraton Polymers, Houston, TX, March 2004. Mitchell, D.M., and Sabia, R., Proceedings of the 29th International Wire and Cable Symposium, Washington, DC, March 1986. Technical Bulletin SC: 1102-89, Shell Chemical Co., Houston, TX, 1989. Drobny, J.G., Paper at the International Rubber Conference, Yokohama, Japan, October 24–28, 2005. Chen, J.Y., U.S. Patents 4,369,284 (January 18, 1983); 5,262,468 (October 21, 1986); and 5,508,344 (April 16, 1996) to Applied Elastomerics, Inc. Holden, G., and Hansen, D.R., in Thermoplastic Elastomers, 3rd edition, chapter 19 (Holden, G., Kricheldorf, H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 508. Haaf, W.R., U.S. Patent 4,167,507 (1990, to General Electric Co.). Paul, D.R., in Thermoplastic Elastomers, 2nd edition, chapter 15C (Holden, G., Legge, N.R., Quirk, R.P., and Schroeder, H.E., Eds.), Hanser Publishers, Munich, 1996. Gilmore, D.W., and Modic, M.J., Plastics Eng. 45(4), p. 51 (1989). Willis, C.L., Halper, W.M., and Handlin, Jr., D.L., Polym. Plast. Technol. Eng. 28(2), p. 207 (1984). Technical Bulletin SC: 1216-91, Shell Chemical Co., Houston, TX, 1991. Polymers for Modifying Bitumen, Technical Information, Kraton Polymers, Houston, TX. Technical Bulletin SC: 1494-93, Shell Chemical Co., Houston, TX, 1993. Holden, G., and Hansen, D.R., in Thermoplastic Elastomers, 3rd edition, chapter 19 (Holden, G., Kricheldorf, H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 509.
30. Rooftop Performance, Fact Sheet K0333 Europe/Africa, Kraton Polymers, Houston, TX, August 2002. 31. Handbook of Thermoplastic Elastomers, 2nd edition (Walker, B.M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York, 1988, p. 131. 32. World Thermoplastic Elastomers, Report, November 2005, Freedonia Group, Cleveland, OH. 33. Handbook of Thermoplastic Elastomers, 2nd edition, chapter 4 (Walker, B.M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York, 1988, p. 92. 34. ASTM D2000, Annual Book of Standards, vol. 19.01, ASTM International. 35. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 178. 36. Handbook of Thermoplastic Elastomers, 2nd edition, chapter 4 (Walker, B.M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York, 1988, p. 132. 37. Rader, C.P., in Handbook of Thermoplastic Elastomers, 2nd edition, chapter 4 (Walker, B. M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York, 1988, p. 110. 38. Handbook of Thermoplastic Elastomers, 2nd edition, chapter 4 (Walker, B.M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York. 39. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 152. 40. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 115. 41. Wallace, J.G., in Handbook of Thermoplastic Elastomers, 2nd edition, chapter 5 (Walker, B. M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York, 1988, p. 167. 42. Hofmann, G.H., and Abell, W.R., in Thermoplastic Elastomers, 3rd edition, chapter 6 (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004. 43. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 131. 44. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 132. 45. Landi, V.R., Appl. Polym. Symp. 25, p. 223 (1974).
46. Hourston, D.J., and Hughes, I.D., J. Appl. Polym. Sci. 26(10), p. 3467 (1981). 47. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 139. 48. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 512. 49. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 37. 50. Schladjewski, R., Schultze, D., and Imbach, K.P., J. Coated Fabrics 27, p. 105 (October 1997). 51. Quinn, F.A., Kapasi, V., and Mattern, R., Paper Presented at the 6th International Conference on Thermoplastic Markets and Products Sponsored by Schotland Business Research, Orlando, FL, March 13–15, 1989. 52. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 513. 53. Bayer Brochure KU 24001, Desmopan ® Texin® , Bayer MaterialScience, Leverkusen, Germany, January 2005. 54. Estane® Overview, Noveon, 2006. 55. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 38. 56. Bonk, H.W., Drzal, R., Georgacopoulos, C., and Shah, T.M., Paper Presented at the Annual Technical Conference of the Society of Plastics Engineers, Washington, DC, 1985. 57. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 514. 58. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 511. 59. Handbook of Thermoplastic Elastomers, 2nd edition, chapter 6 (Walker, B.M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York. 60. Handbook of Thermoplastic Elastomers (Walker, B.M., Ed.), chapter 4, Van Nostrand Reinhold, New York. 61. Plastics.dupont.com. 62. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 212. 63. Handbook of Thermoplastic Elastomers, 2nd edition, chapter 6 (Walker, B.M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York, p. 212.
64. Handbook of Thermoplastic Elastomers, 2nd edition (Walker, B.M., and Rader, C.P., Eds.), chapter 6, Van Nostrand Reinhold, New York, p. 222. 65. Wang, S., Polym. J. (Tokyo) 21, p. 179 (1989). 66. Bakker, D., et al., J. Biomed. Mater. Res. 24, p. 277 (1990). 67. Vrovenraets, C.M.F., and Sikema, D.J., U.S. Patent 4,493, 870 (January 15, 1985, to Akzo); Ostapchenko, G.J., U.S. Patent 4,725,481 (February 16, 1988, to DuPont). 68. Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 242. 69. Reeves, N., Paper Presented at the Conference TPE ’98, New Opportunities for Thermoplastic Elastomers, London, UK, November 30, December 1, 1998. 70. Pebax® Application Areas, Publication DIREP 3200/06.2000/30, ATOFINA, Puteau, France, 2000. 71. Degussa High Performance Polymers Vestamid® , Publication 02/gu/1500/e, Degussa, AG, Marl, Germany. 72. Handbook of Thermoplastic Elastomers, 2nd edition, chapter 6 (Walker, B.M., and Rader, C.P., Eds.), Van Nostrand Reinhold, New York, p. 282. 73. McCoy, J., Elastomers, Gaskets and Seals: Scratching the Surface, Appliance Design Magazine, June 2005. 74. MacKnight, W.J., and Lundberg, R.D., in Thermoplastic Elastomers, 3rd edition, chapter 11 (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004. 75. Kar, K.K., and Bhowmick, A.K., in Handbook of Elastomers, 2nd edition, (Bhowmick, A.K., and Stephens, H.L., Eds.), Marcel Dekker, New York, 2001. 76. Duvdevani, I., et al., U.S. Patent 4,701,204 (October 20, 1987, to Exxon Research and Engineering).
77. Plastics Technology, Ionomer-Based TPEs Are Scratch and Mar Resistant, Online Article, November 2005. 78. McCoy, J., and Sadeghi, R., Development of New Soft Touch Thermoplastic Elastomers Based on Ionomer Polymer, 56th Annual International Appliance Technical Conference and Exhibition, March 28–30, 2005, Rosemont, Illinois. 79. Ecker, R., U.S. Patent 4,116,917 (1978). 80. Arie, V.Z., and Jacoba Gerarda, European Patent 200,679 (1991). 81. Charles, C., Shiaw, J., and Ver Strate, G., U.S. Patent 813,848 (1985). 82. Struglinski, M.J., Ver Strate, G., and Fetters, L.J., U.S. Patent 670,114 (1991). 83. Robert, J.S., and Robert, B.R., U.S. Patent 100,656 (1993). 84. Mishra, M.K., and Saxton, R.G., Chem. Tech. 35 (1995). 85. Diehl, C.F., et al., U.S. Patent 5,399,627 (1995, to the Dow Chemical Company and Exxon Chemical Patents, Inc.). 86. Himes, G.R., et al., U.S. Patent 5,639,831 (1997, to Shell Oil Co.). 87. Naylor, F.E., U.S. Patent 3,932,327 (1976, to Phillips Petroleum Co.). 88. Simms, J.A., Rubber Chem. Technol. 64, p. 139 (1991). 89. Simms, J.A., Progr. Org. Coatings 22, p. 367 (1993). 90. Simms, J.A. and Spinnelli, H.J., J. Coat. Technol. 59, p. 125 (1987). 91. Shim, J.S., and Kennedy, J.P., Polym. Prepr. 39(2), p. 617 (1998). 92. Gergen, W.P., and Davison, S., U.S. Patent 4,101, 605 (July 18, 1978, to Shell Oil). 93. Sperling, L.H., in Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 435. 94. Sperling, L.H., in Thermoplastic Elastomers, 3rd edition (Holden, G., Kricheldorf., H.R., and Quirk, R.P., Eds.), Hanser Publishers, Munich, 2004, p. 440.